Nanopowder Metal Oxide for Photoluminescent Gas Sensing
© The Author(s). 2017
Received: 29 December 2016
Accepted: 17 January 2017
Published: 20 February 2017
Gas sensing properties of metal oxide nanopowders (ZnO, TiO2, WO3, SnO2) with average diameters of 40–60 nm were analyzed by room-temperature photoluminescence spectroscopy. The influence of gas environment (O2, N2, H2, CO, CO2) on the emission intensity was investigated for metal oxide nanopowders with surface doped by impurities (Pt, Ag, Au, Sn, Ni or Cu). Established physicochemical regularities of modification of surface electronic states of initial and doped nanopowders during gas adsorption. The nature of metal oxide nanopowder gas-sensing properties (adsorption capacity, sensitivity, selectivity) has been established and the design and optimal materials for the construction of the multi-component sensing matrix have been selected.
Sensors for active, in particular, toxic and explosive gases play an important role in the monitoring and control of the environment, especially in highly industrialized regions. Gas sensors based on nanostructured metal oxides have shown great potential for the detection of different gases, in particular, toxic, hazardous, or inflammable gases such as H2, CO, NO2 or NH3 [1–3]. Such sensors can also be applied in medicine, particularly for diagnosis of cancer . Nanopowders have excellent sensing properties due to their high surface-to-volume ratio [5, 6], which has high adsorption ability and reactivity . Among semiconductor sensors, metal oxide nanopowders are of interest as nontoxic, easy-to-handle, and highly sensitive materials that can be grown with excellent crystal quality using different physical and chemical fabrication techniques [8–12]. In addition, the use of different cover metal layers (Pt, Ag, Au, Sn, Ni or Cu) as catalysts for gas chemisorption or physisorption can achieve an increase in the detection limit for specific gases and could be in the range of parts per billion (ppb) [13–15].
Gas sensing is performed mostly by electrical measurement. The adsorption of oxidative and reductive gases on the surface of nanopowders leads to a change in the charge density on the surface and a shift of the Fermi level. This induces a change in the electron distribution in the nanomaterial [16–18]. A wide range of adsorption centers leads to low selectivity of material, and consequently we need to find ways of improving this. The difficulty of selective detection is due to in particular to a similar mechanism of interaction of the reductant gases with the surface of metal oxides. The sensitivity of metal oxides to the nature and concentration of adsorbed molecules largely depends on the surface microstructure, which can be modified both by laser annealing and by the formation of complex heterogeneous systems, including the metal-semiconductor type “core-shell” . The solution to this problem can also be to use arrays of metal oxide nanopowders covered with different functional additives that affect the adsorption process .
Several publications on luminescent gas sensing are available [18–25]. An advantage of luminescent sensing is that it avoids electrical contact between the nanostructures and the resulting metallic impurities. Also, real-time information about the change of specific contributions in the photoluminescence spectra can be observed. However, the direct effect of adsorbed gases on the photoluminescence of metal oxide nanopowders has not yet been adequately studied.
This work aims at solving the problem of increasing the selectivity of the gas-sensitive materials and accordingly, gas sensors in general. Its feature is an integrated approach to solving problems that is to use the methods of fabrication of nanopowders and structures on the basis that we have developed [19, 21, 26] and to apply the photoluminescent method for the detection of adsorbed gas particles on the surface of metal oxide nanopowders [20, 21]. This approach is promising due to its very high inherent sensitivity and miniaturization capability.
The research into phase and structural analyses of nanopowders was carried out using an x-ray diffractometer, DRON-4. The sizes of particles were determined according to electron microscopy images received by means of the electron microscope, PEM-125 K.
Doping of nanopowders was conducted by pulsed laser deposition of thin films on the nanopowders with further activation by laser annealing [27, 28]. Pulsed evaporation of target material was carried out using a neodymium-doped yttrium aluminium garnet (Nd:YAG) laser (λ = 1,06 μm, τ = 10-3–10-8 s, q = 105÷108 W/cm2, n = 14–56 Hz, d = 5 mm, Ei = 0.005–0.350 J). Laser radiation was focused on the target located in a vacuum chamber (P = 10-3 Pa), so we obtained chemically pure condensates of activator. The plasma plume was directed perpendicular to the nanopowder level in the cuvette. Dopant atoms condensed on the surface of the powder and formed the thin film of dopant. The cuvette containing the nanopowder was placed on the vibration device (oscillation frequency 10–60 Hz); this provided an even film of condensation over the entire surface of the nanopowder. The vibrating oscillations provide good mixing of powder, allowing even deposition of film on its surface. With the purpose of activating the deposited impurities and its diffusely uniform distribution in the volume of granule was carried out laser annealing of nanopowder. Under the action of pulsed laser emission the alloying metallic impurities from the surface diffuses into granules and is electrically activated. Laser heating and implantation carried out in the transparency band of nanopowders and therefore with the absorption of radiation on the metallic impurity and without significant heating of nanopowders.
Photoluminescent research into gas environments were conducted using the computerized device with the dual monochromator DMR-4. Photoluminescence excitation was performed using UV light-emitting diodes (LEDs) with λmax = 355 or λmax = 375 nm. The photoluminescent study was carried out at room temperature. The investigated samples were placed in a quartz cuvette connected to the vacuum installation VUP-5 M and the multi-system gas inlet SNA-2, which made it possible to conduct photoluminescent research in various gas environments at a given range of pressures. Registration of the signal was carried out using the photomultiplier FEU-27. Recording and normalization of spectra was conducted automatically using specially developed software.
Results and Discussion
The metal oxide nanopowder samples were obtained by means of pulse laser-reactive technology [17, 19]. X-ray diffraction studies show that ZnO samples have a wurtzite crystal structure and an average diameter of nanoparticles of 40–60 nm.
The influence of the deposited catalysts on the sensitivity and selectivity of the semiconductor sensors can also be shown through adsorption and change in the characteristics of the space charge region, which is located directly under contact with the catalytic metallic impurity – the semiconductor, caused by adsorption. The processes that occur during adsorption on metal impurities cause changes in the electronic subsystem and changes in the characteristics of the Schottky barrier, which is demonstrated by changes in the concentration of free carriers in the space charge region that participate in the luminescent process.
The observed increase in the sensitivity of ZnO nanoparticles to oxygen is probably caused by the combination of two effects, namely electronic sensitization and as a result of this, the effect of platinum on the surface of metal oxide ZnO. Sensitization is due to differences in the work function between regions of covered platinum and uncovered ZnO nanoparticles. In comparison with ZnO, platinum has a higher value of work function. This means that the Fermi level of ZnO nanoparticles is lower than for platinum, which leads to the transfer of some free electrons from ZnO nanoparticles to the platinum cover, as both systems achieve thermodynamic equilibrium, changing the position of the Fermi level.
Reducing the number of free electrons in ZnO nanoparticles causes an increase in the thickness of the depletion layer . The spillover effect causes increased dissociation of oxygen molecules to oxygen ions. Thus, a weak coupling is formed between the oxygen molecule and the platinum atom. This weak coupling can be easily broken with the formation of oxygen ions that diffuse to the surface vacancies of ZnO nanoparticles. Thus, there are more trapped electrons, which increase the sensitivity of ZnO nanoparticles to gases. The mechanism of the catalytic ability of gold on the surface of ZnO nanoparticles can be twofold. On the surface of a gold cluster there is active interaction of oxygen with gold and additional activation of chemisorbed oxygen on the border of the three-phase system, Au-ZnO-O2.
The sensor system predicted by us is based on the registration photoluminescence spectra of metal oxide nanopowder with adsorbed gas particles . The energy levels of electrons are created in the adsorbent by adsorbed particles, which allow us to observe individual electron spectral levels of the adsorbed atoms and selectively identify them.
The luminescent properties of metal oxide nanopowders (ZnO, TiO2, SnO2, WO3) have been studied in various gas environments (O2, N2, H2, CO, CO2) for use in gas sensing. The effect on gas sensing properties (adsorption capacity, sensitivity and selectivity) of a surface doped by impurities (Pt, Ag, Au, Sn, Ni or Cu) was investigated. We proposed a multichannel luminescent sensor system, which has a set of metal oxide adsorbents of various modifications, which are characterized by different sensitivity to various gas particles. Simultaneous measurements of the luminescent signals of cells in this system provide an opportunity to determine the qualitative and quantitative composition of the components in the gas environment.
All the authors took part in solving the problem under study. They read and approved the manuscript.
The authors declare that they have no competing interests.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Arafat MM, Dinan B, Akbar SA, Haseeb ASMA (2012) Gas sensors based on one dimensional nanostructured metal-oxides: a review. Sensors 12(6):7207–7258. doi:10.3390/s120607207 View ArticleGoogle Scholar
- Comini E (2006) Metal oxide nano-crystals for gas sensing. Anal Chim Acta 568(1-2):28–40. doi:10.1016/j.aca.2005.10.069 View ArticleGoogle Scholar
- Yamazoe N (2005) Toward innovations of gas sensor technology. Sens Actuators B 108:2–14. doi:10.3390/s120607207 View ArticleGoogle Scholar
- Simon E (2010) Biological and chemical sensors for cancer diagnosis. Meas Sci Technol 21(11):112002. doi:10.1088/0957-0233/21/11/112002 View ArticleGoogle Scholar
- Sun Y-F, Liu S-B, Meng F-L, Liu J-Y, Jin Z, Kong L-T, Liu J-H (2012) Metal oxide nanostructures and their gas sensing properties: a review. Sensors 12(3):2610–2631. doi:10.3390/s120302610 View ArticleGoogle Scholar
- Wei A, Pan L, Huang W (2011) Recent progress in the ZnO nanostructure-based sensors. Mater Sci Eng B 176(18):1409–1421. doi:10.1016/j.mseb.2011.09.005 View ArticleGoogle Scholar
- Wang C, Yin L, Zhang L, Xiang D, Gao R (2010) Metal oxide gas sensors: sensitivity and influencing factors. Sensors 10(3):2088–2106. doi:10.3390/s100302088 View ArticleGoogle Scholar
- Zhong LW (2004) Zinc oxide nanostructures: growth, properties and applications. J Phys Condens Matter 16:R829–R858. doi:10.1088/0953-8984/16/25/R01 View ArticleGoogle Scholar
- Kotlyarchuk BK, Popovych DI, Savchuk VK, Serednycki AS (2003) Pulsed laser deposition of ZrO2 thin films for application in microelectronic devices. Phys Chem Solid State 4(3):434–439Google Scholar
- Kabashin AV, Delaporte P, Pereira A, Grojo D, Torres R, Sarnet T, Sentis M (2010) Nanofabrication with pulsed lasers. Nanoscale Res Lett 5(3):454–463. doi:10.1007/s11671-010-9543-z View ArticleGoogle Scholar
- Olenych IB (2016) Effect of ZnO layers on transport and relaxation of charge in porous silicon–silicon structures. Nanosci Nanoengineering 83(1):111–114. doi:10.13189/nn.2016.040202 Google Scholar
- Foo KL, Hashim U, Muhammad K, Voon CH (2014) Sol–gel synthesized zinc oxide nanorods and their structural and optical investigation for optoelectronic application. Nanoscale Res Lett 9(1):429. doi:10.1186/1556-276X-9-429 View ArticleGoogle Scholar
- Anderson T, Ren F, Pearton S, Kang BS, Wang H-T, Chang C-Y, Lin J (2009) Advances in hydrogen, carbon dioxide, and hydrocarbon gas sensor technology using GaN and ZnO-based devices. Sensors 9(6):4669–4694. doi:10.3390/s90604669 View ArticleGoogle Scholar
- Daryakenari AA, Apostoluk A, Delaunay J-J (2013) Effect of Pt decoration on the gas response of ZnO nanoparticles. Phys Status Solidi C 10(10):1297–1300. doi:10.1002/pssc.201200937 Google Scholar
- Tamaekong N, Liewhiran C, Wisitsoraat A, Phanichphant S (2009) Sensing characteristics of flame-spray-made Pt/ZnO thick films as H2 gas sensor. Sensors 9(9):6652–6669. doi:10.3390/s90906652 View ArticleGoogle Scholar
- Bovgyra OV, Bovgyra RV, Popovych DI, Serednytski AS (2015) The density functional theory study of electronical properties of (ZnO)12 clusters during gas adsorption. J Nano Electron Physics 7(4):04090(6)Google Scholar
- Bovgyra OV, Bovgyra RV, Kovalenko MV, Popovych DI, Serednytski AS (2013) The density functional theory study of structural and electronical properties of ZnO clusters. J Nano Electron Physics 5(1):01027(6)Google Scholar
- Madel M, Jakob J, Huber F, Neuschl B, Bauer S, Xie Y, Tischer I, Thonke K (2015) Optical gas sensing by micro-photoluminescence on multiple and single ZnO nanowires. Phys Status Solidi A 8:1810–1816. doi:10.1002/pssa.201431688 View ArticleGoogle Scholar
- Gafiychuk VV, Ostafiychuk BK, Popovych DI, Popovych ID, Serednytski AS (2011) ZnO nanoparticles produced by reactive laser ablation. Appl Surf Sci 257:8396–8401. doi:10.1016/j.apsusc.2011.04.084 View ArticleGoogle Scholar
- Bovhyra RV, Zhyrovetsky VM, Popovych DI, Savka SS, Serednytsky AS (2016) Development and creating of gas-sensor system based on low dimensional metal oxides. Nauka Innov 12(6):59–65. doi:10.15407/scin12.06.059 View ArticleGoogle Scholar
- Kotlyarchuk BK, Myronyuk IF, Popovych DI, Serednytski AS (2006) Synthesis of oxide nanopowder materials and research of their luminescent properties. Phys Chem Solid State 7(3):490–494Google Scholar
- Comini E, Baratto C, Faglia G, Ferroni M, Sberveglieri G (2007) Single crystal ZnO nanowires as optical and conductometric chemical sensor. J Phys D Appl Phys 40(23):7255–7259. doi:10.1088/0022-3727/40/23/S08 View ArticleGoogle Scholar
- Setaro A, Bismuto A, Lettieri S, Maddalena P, Comini E, Bianchi S, Baratto C, Sberveglieri G (2008) Optical sensing of NO2 in tin oxide nanowires at sub-ppm level. Sens Actuators B 130(1):391–395. doi:10.1016/j.snb.2007.09.015 View ArticleGoogle Scholar
- Maier K, Helwig A, Muller G, Becker P, Hille P, Schormann J, Teubert J, Eickhoff M (2014) Detection of oxidising gases using an optochemical sensor system based on GaN/InGaN nanowires. Sens Actuators B 197:87–94. doi:10.1016/j.snb.2014.02.002 View ArticleGoogle Scholar
- Valerini D, Creti A, Caricato AP, Lomascolo M, Rella R, Martino M (2010) Optical gas sensing through nanostructured ZnO films with different morphologies. Sensors Actuators B 145(1):167–173. doi:10.1016/j.snb.2009.11.064 View ArticleGoogle Scholar
- Ostafiychuk BK, Zhurovetski VM, Kotlyarchuk BK, Moysa MI, Popovych DI, Serednytski AS (2008) Synthesis of investigation of properties and synthesis processes of nanopowder ZnO. Phys Chem Solid State 9(4):728–731Google Scholar
- Shevchuk VN, Popovych DI, Belyukh VM, Usatenko YN (2013) Specifics of the diffuse reflectance spectra of TiO2 nanopowders doped by 3d-ions. Nanosystems Nanomater Nanotechnol 11(1):99–108Google Scholar
- Kovalyuk B, Kovalyuk B, Mocharskyi V, Yu N, Onisimchuk V, Popovych D, Serednytski A, Zhyrovetsky V (2013) Modification of structure and luminescence of ZnO nanopowder by the laser shock-wave treatment. Phys Status Solidi C 10:1288–1291. doi:10.1002/pssc.201200889 Google Scholar
- Boudart M (1952) Electronic Chemical Potential in Chemisorption and Catalysis. J Amer Chem Soc 74(6):1531–1535. doi:10.1021/ja01126a055 View ArticleGoogle Scholar